# Characterizing the Local Primary Dendrite Arm Spacing in Directionally Solidified Dendritic Microstructures

- 1.2k Downloads
- 7 Citations

## Abstract

Characterizing the spacing of primary dendrite arms in directionally solidified microstructures is an important step for developing process–structure–property relationships by enabling the quantification of (i) the influence of processing on microstructure and (ii) the influence of microstructure on properties. In this work, we utilized a new Voronoi-based approach for spatial point pattern analysis that was applied to an experimental dendritic microstructure. This technique utilizes a Voronoi tessellation of space surrounding the dendrite cores to determine nearest neighbors and the local primary dendrite arm spacing. In addition, we compared this technique to a recent distance-based technique and a modification to this using Voronoi tessellations. Moreover, a convex hull-based technique was used to include edge effects for such techniques, which can be important for thin specimens. These methods were used to quantify the distribution of local primary dendrite arm spacings, their spatial distribution, and their correlation with interdendritic eutectic particles for an experimental directionally solidified Ni-based superalloy micrograph. This can be an important step for correlating processing and properties in directionally solidified dendritic microstructures.

## 1 Introduction

Developing an enhanced understanding of mechanical behavior in materials relies upon sufficiently characterizing microstructure details at the relevant length scales that contribute to this behavior. Moreover, to truly enhance the predictive capability of processing–structure–property models that aim to improve material performance requires a quantitative stereological description of the relevant microstructure features and, thereby, the material itself. Predictive models that effectively capture the linkage between processing and properties (through microstructure) can be utilized within an integrated computational materials engineering (ICME) approach to design materials and accelerate their insertion into application.

The focus of the present work is on single-crystal nickel-based superalloys, which are used in turbine blades within the high temperature section of the modern turbine engine.[1,2] In single-crystal nickel-based superalloys, there are a number of length scales of microstructure that contribute to mechanical behavior, ranging from the \(\gamma^\prime\) precipitates to pores and eutectic particles to the dendrites themselves. At the largest microstructure length scale in directionally solidified single-crystal microstructures, the features of interest are the dendrites; many features at lower length scales (*e.g.*, eutectic particles, precipitates, *etc.*) or at similar scales (*e.g.*, porosity, freckle defects, *etc.*) are strongly associated with the dendrite arm spacing and morphology.[3, 4, 5, 6, 7] The solidification morphology associated with dendrite arm spacing has been described in the literature.[8,9] Historically, the primary dendrite arm spacing (PDAS) has been found to correlate with processing (*e.g.*, solidification rate)[7,10, 11, 12, 13, 14] as well as with properties (*e.g.*, creep strength, fatigue properties).[15,6] For instance, Lamm and Singer[6] produced single-crystal nickel-based microstructures (PWA 1483) with a varied range of different dendrite arm spacings (250 to 600 *μ*m) and found that decreasing the mean dendrite arm spacing was associated with an increased high-cycle fatigue life. The fatigue cracks were found to originate at shrinkage porosity and the largest pores correlated with a large PDAS.

*λ*is PDAS,

*A*is the area analyzed,

*n*is the number of dendrites, and

*c*is a coefficient that depends on the microstructure. McCartney and Hunt[10] showed that

*c*= 0.5 for a random array of points,

*c*= 1 for a square array of points, and

*c*= 1.075 for a hexagonal array of points; they had to apply a correction for the bulk dendrite arm spacing

*λ*as processing conditions caused a change in the local environment of the dendrites. However, this approach is insufficient for capturing local arm spacings or the dendrite arm spacing distribution, and may provide problems with complex geometries such as turbine blades. In fact, part of the motivation for quantifying the local PDAS is that a narrow distribution (

*i.e.*, low standard deviation) of local PDAS values may result in a more homogeneous distribution of interdendritic microstructure features and, more importantly, a narrow distribution of mechanical properties.[18] For instance, structural inhomogeneities in single-crystal components, which may cause wider property variations, have been correlated to asymmetric heat flux and transients in solidifications.[19]

The research objective herein is to evaluate the capability of some recent approaches, as well as some modified versions of these approaches, for characterizing the local dendrite arm spacing within experimental dendritic microstructures. In this work, an experimental dendritic microstructure is used for this analysis along with three different techniques that are based on the nearest neighbor spacing and/or a Voronoi tessellation of the dendrite cores. Comparison of existing and new metrics with traditional PDAS metrics is discussed for both local and global measures. The current methods investigated supply statistical information of local spacing and coordination number while introducing a technique for addressing edge effects and examining the parameter sensitivity of these different methods. In comparison to previous work,[20] this work introduces and compares the statistical distributions of local dendrite arm spacings for the four methods, for a more quantitative analysis. It was found that augmenting existing techniques with Voronoi tessellations to define the subset of first nearest neighbors or refining existing Voronoi-based techniques resulted in a more physical description of the local dendrite arm spacing. Moreover, for certain cases, the mean local dendrite statistics can adequately approximate the PDAS found with the traditional bulk characterization technique (Eq. [1]).

## 2 Methodology

*a*

_{0}noise fraction[2]), as shown in Figure 1(a).[20] For the purposes of describing several different methods shown in Figure 1, this synthetic pattern of points can be considered as the cores of primary dendrites.

One such method for measuring the local dendrite arm spacing is the Warnken–Reed method.[21,22] The Warnken–Reed method calculates the dendrite arm spacing for a single point (black dot) by starting with an initial number of nearest neighbors, *k*_{initial}, (3 closest neighbors) and iteratively adding potential nearest neighbors that are within a cutoff distance defined by the already-added nearest neighbors. For instance, the inner circle in Figure 1(b) represents the average spacing, *d*_{avg}, of these neighbors and the outer circle represents the cutoff for adding the next neighbor, *d*_{avg} + *αd*_{std}, where *d*_{std} is the standard deviation of the nearest neighbor spacings and *α* is a parameter that is typically between 1 and 2. Neighbors continue to be added until the cutoff does not include any new neighbors. The local coordination number and dendrite arm spacing is calculated from the neighbors added (shown as red dots). However, if the standard deviation of the distances of the nearest neighbors *d*_{std} or the parameter *α* is large, this technique can continue to add nearest neighbors beyond the first nearest neighbors; our implementation stopped after 20 nearest neighbors. Clearly, a method for restricting the number of nearest neighbors using such a technique is necessary.

A simple way of identifying the potential first nearest neighbors is to perform a Voronoi tessellation of the space surrounding the points, as shown in Figure 1(c). The polygon edges are equidistant between the points contained in the two adjacent polygons and the triple points (merging of three lines) are equidistant between the points contained in the three adjacent polygons. Therefore, the first nearest neighbors (FNNs, shown as open circles in Figure 1(c)) correspond to the edges of the central polygon (that contains the black dot). This subset of points is the maximum number of nearest neighbors that the central point can have.

In this manner, several techniques have been identified to quantify a local dendrite arm spacing based on the Voronoi-identified FNNs.[20] For instance, the Voronoi Warnken–Reed method (Figure 1(d)) only includes the Voronoi FNNs as potential nearest neighbors and cannot expand beyond these, alleviating a potential problem of selecting second nearest neighbors or greater. Another method using the Voronoi FNNs is to consider all of these potential nearest neighbors as nearest neighbors (Figure 1(e)), as in Brundidge *et al.*[14] Unfortunately, this approach is sensitive to small perturbations in the spatial positions of the neighbors. For instance, if the lower right hand neighbor in Figure 1(e) moves away from the central point, it no longer shares an edge with the polygon containing the black dot; in this scenario, the two adjacent polygons on either side effectively “pinch” off this neighbor. This scenario, however, has a physical basis as these two dendrite cores mainly compete with the central core, and the lower right core has a much less prominent effect on the central core. The last method, which is examined in the present paper, utilizes a criterion based on the edge lengths of the Voronoi polygon. In Figure 1(f), those neighbors with edge lengths less than a critical fraction, *d*_{crit}, of the total polygon perimeter are excluded as nearest neighbors (*e.g.*, 10 pct in Figure 1(f)). In the present study, the local dendrite arm spacing statistics are evaluated using these four techniques: Warnken–Reed, Voronoi Warnken–Reed, and the Voronoi technique with (*d*_{crit} > 0) and without (*d*_{crit} = 0) a line length threshold.

*d*

_{std}value from the initial three distances. The Voronoi-modified version in Figure 2(d) stops at four nearest neighbors despite the fact that several points lie within the outer boundary computed by this method. The Voronoi method with

*d*

_{crit}= 0.0 clearly overestimates the number of nearest neighbors, while the four nearest neighbors identified through

*d*

_{crit}= 0.10 (Figure 2(f)) perhaps offers a better approximation of the number of nearest neighbors. Interestingly, comparing the methods in Figures 2(d) and (f), the coordination number is the same, but the nearest neighbors identified is different. This is due to the Warnken–Reed method being a distance-based method, and identifying the four closest neighbors, while the modified Voronoi technique is based on the edge lengths of the Voronoi polygon, and hence utilizes this to identify nearest neighbors (which may not be the closest neighbors).

The traditional PDAS metric does not consider the order or disorder of the dendrites within the microstructure. Figure 2 illustrates why a local metric for PDAS may be needed. For the field of view given in Figures 1(a) and 2(a), the bulk PDAS metric would be the same since the number of dendrites *n* and the area *A* are equal (see Eq. [1]). However, the disorder of the dendritic structure in the case of Figure 2 may yield (i) a more uneven distribution of solute elements, (ii) the formation of second phase particles, (iii) the formation of gas or shrinkage porosity, or (iv) the lateral growth of secondary dendrite arms. Hence, in addition to the bulk PDAS values, understanding how processing conditions may impact the disorder of the dendritic structure may be important for understanding the properties of directionally solidified alloys.

*m*) and the standard deviation (

*σ*) characterize the disorder of the system and casting these values into a

*m*-

*σ*design space allows for comparison between different point systems.[23] This has been effectively applied to characterize the mean dendrite arm spacing, PDAS distribution, and the disorder in first Pb-Tl alloys[24] and subsequently in other alloy systems.[11,18,25] As an example of this technique, Figure 3 plots the dendrite cores and connecting line segments for the single-crystal nickel-based superalloy micrograph used in this study (Figure 4). Moreover, other methods such as radial distribution functions, fast Fourier transforms, and/or correlation functions can also be used to characterize the dendrite arm spacing distribution. However, it should be noted that these approaches are not intended for local characterization of the dendrite arm spacing and are not as effective for correlating the local spacing with local microstructure features as shown herein. Moreover, these techniques do not quantify the number of nearest neighbors and are often coupled with Voronoi polygons to compute the nearest neighbor distributions. Rather, these analysis methods are more effective at characterizing and comparing the homogeneity/heterogeneity of the dendritic structure between different processing conditions. Hence, there will be limited discussion of these techniques in the present work.

## 3 Results

### 3.1 Application to Dendritic Microstructure

A micrograph of a directionally solidified single-crystal nickel-based superalloy microstructure that is polished and imaged perpendicular to the solidification direction is shown in Figure 4. This microstructure was produced using the liquid metal cooling technique, as described in Miller[26] and Elliott *et al.*[4] First, the dendrite cores were identified manually (white and black dots). Automated methods to identify dendrite cores can be invaluable for future large scale analysis.[27,28] Moreover, the white particles in this image are eutectic particles. A total of 393 dendrite cores are contained in this image over an area of 24.25 mm^{2}, giving a PDAS of 248.4 *μ*m using *c* = 1 (Eq. [1]). The remainder of the analysis uses this micrograph as a template for characterizing the local dendrite arm spacing.

### 3.2 Accounting for Image/Part Edge Effects

### 3.3 Spatial Distribution of Local Primary Dendrite Arm Spacings

*d*

_{crit}= 0.12. Dendrite cores with local PDAS similar to the mean PDAS of the bulk (248.4

*μ*m) are colored white and those with PDAS above (below) the mean PDAS are red (blue); the lower and upper bounds of the color bar are −25 and +25 pct of the mean PDAS value, respectively. In general, the exterior dendrite cores have similar PDAS as the interior dendrite cores using this technique. A similar color bar is used for the coordination number as well. As would be expected, the exterior dendrite cores tend to have a lower coordination number than the interior dendrite cores, with a few that only have 2 nearest neighbors. However, the dendrite cores with a low coordination number on the edges are not consistently over/under the mean PDAS (

*i.e.*, they do not significantly bias the statistics from the edge dendrite cores). Future work will examine what techniques may be most applicable for characterizing local dendrite arm spacings and coordination numbers for dendrite cores on free surfaces. It is envisioned that sectioning large numbers of instantiations of synthetically generated microstructures of known bulk dendrite arm spacings can be used to understand the bias introduced by edge effects and to understand what are the best techniques for quantifying the local spacing.

*d*

_{crit}= 0.0 has a much larger fraction of dendrite cores with PDAS greater than the bulk PDAS than below the bulk PDAS (83.5 pct above 248.4

*μ*m). Clearly, the local PDAS is overpredicted in this case. The Warnken–Reed and Voronoi Warnken–Reed methods are shown in Figures 7(b) and (c). At first glance, a majority of the local PDAS values are very similar between the two methods (∼79 pct). However, ∼21 pct of the cores resulted in a difference between the two techniques, which is caused by the original Warnken–Reed method using neighbors outside of those FNNs identified from the Voronoi polygons. In every case, the Warnken–Reed method resulted in higher local PDAS values than the Voronoi Warnken–Reed method, as would be expected since this is purely a distance-based method and subsequent additions can only increase the local PDAS.

*μ*m and/or 100 pct of the PDAS value quantified by the Voronoi Warnken–Reed method. The differing dendrite cores is approximately an equal percentage for edge dendrites as well as interior dendrite cores.

### 3.4 Local Primary Dendrite Arm Spacing Statistics

Local Primary Dendrite Arm Spacing Statistics

Method | Parameter | Primary Dendrite Arm Spacing | ||||
---|---|---|---|---|---|---|

Mean ( | Diff. (Pct) | Std ( | Skewness | Kurtosis | ||

Bulk (Eq. [1], | — | 248.4 | 0.0 | — | — | — |

Voronoi Tessellation |
| 272.9 | 9.9 | 28.0 | 0.1 | 3.3 |

Voronoi Tessellation |
| 270.0 | 8.7 | 27.2 | 0.1 | 3.2 |

Voronoi Tessellation |
| 266.4 | 7.2 | 26.8 | 0.1 | 3.1 |

Voronoi Tessellation |
| 263.0 | 5.9 | 25.7 | 0.1 | 3.1 |

Voronoi Tessellation |
| 258.4 | 4.0 | 26.1 | 0.2 | 3.1 |

Voronoi Tessellation |
| 253.3 | 2.0 | 25.3 | 0.2 | 3.0 |

Voronoi Tessellation |
| 247.6 | −0.3 | 26.0 | 0.2 | 2.9 |

Voronoi Warnken–Reed |
| 230.0 | −7.4 | 25.0 | 0.4 | 3.5 |

Voronoi Warnken–Reed |
| 230.9 | −7.0 | 26.0 | 0.4 | 3.4 |

Voronoi Warnken–Reed |
| 232.7 | −6.3 | 27.4 | 0.4 | 3.2 |

Voronoi Warnken–Reed |
| 236.1 | −5.0 | 29.5 | 0.4 | 3.1 |

Voronoi Warnken–Reed |
| 239.0 | −3.8 | 30.5 | 0.4 | 3.0 |

Voronoi Warnken–Reed |
| 242.2 | −2.5 | 31.8 | 0.3 | 3.0 |

Warnken–Reed |
| 230.1 | −7.4 | 25.1 | 0.3 | 3.4 |

Warnken–Reed |
| 231.8 | −6.7 | 26.9 | 0.5 | 3.5 |

Warnken–Reed |
| 234.5 | −5.6 | 29.4 | 0.6 | 3.8 |

Warnken–Reed |
| 239.2 | −3.7 | 33.0 | 0.8 | 4.0 |

Warnken–Reed |
| 248.1 | −0.1 | 48.1 | 1.9 | 8.3 |

Warnken–Reed |
| 259.2 | 4.3 | 64.2 | 1.9 | 6.5 |

Minimal Spanning Tree | N/A | 215.2 | −13.4 | 34.1 | −0.5 | 4.8 |

Local Coordination Number Statistics

Method | Parameter | Coordination Number (Pct) | Mean | ||||
---|---|---|---|---|---|---|---|

3 | 4 | 5 | 6 | ≥7 | |||

Voronoi Tessellation |
| 0.0 | 2.5 | 20.4 | 57.3 | 19.8 | 5.98 |

Voronoi Tessellation |
| 0.0 | 4.0 | 26.0 | 57.0 | 13.0 | 5.80 |

Voronoi Tessellation |
| 0.0 | 7.4 | 34.7 | 51.4 | 6.5 | 5.57 |

Voronoi Tessellation |
| 0.0 | 11.8 | 45.2 | 39.9 | 3.1 | 5.35 |

Voronoi Tessellation |
| 1.5 | 24.1 | 49.2 | 24.8 | 0.3 | 4.98 |

Voronoi Tessellation |
| 5.3 | 43.0 | 41.5 | 10.2 | 0.0 | 4.57 |

Voronoi Tessellation |
| 17.3 | 52.3 | 26.9 | 3.4 | 0.0 | 4.16 |

Voronoi Warnken–Reed |
| 94.1 | 4.6 | 0.9 | 0.0 | 0.3 | 3.08 |

Voronoi Warnken–Reed |
| 87.6 | 8.7 | 2.8 | 0.3 | 0.6 | 3.18 |

Voronoi Warnken–Reed |
| 79.3 | 11.8 | 5.3 | 2.5 | 1.2 | 3.35 |

Voronoi Warnken–Reed |
| 65.9 | 18.0 | 8.0 | 5.3 | 2.8 | 3.62 |

Voronoi Warnken–Reed |
| 56.3 | 19.8 | 12.1 | 8.4 | 3.4 | 3.84 |

Voronoi Warnken–Reed |
| 48.6 | 19.8 | 14.9 | 11.5 | 5.3 | 4.07 |

Warnken–Reed |
| 91.6 | 7.1 | 0.9 | 0.0 | 0.3 | 3.10 |

Warnken–Reed |
| 83.9 | 9.6 | 4.0 | 1.2 | 1.2 | 3.27 |

Warnken–Reed |
| 72.8 | 14.6 | 7.1 | 2.8 | 2.8 | 3.52 |

Warnken–Reed |
| 58.5 | 21.7 | 9.0 | 4.0 | 6.8 | 3.89 |

Warnken–Reed |
| 52.0 | 19.2 | 10.8 | 6.2 | 11.8 | 4.63 |

Warnken–Reed |
| 44.0 | 19.2 | 12.1 | 7.1 | 17.6 | 5.55 |

There are distinct differences between the local dendrite arm spacing distributions calculated by the four techniques (Figure 9 and Table I). The Warnken–Reed and Voronoi Warnken–Reed are compared initially. In the case of the Warnken–Reed method, the PDAS distribution is shifted towards large PDAS values at high *α* values (a positive skewness value gives a long tail) and has a sharper peak and a longer, fatter tail (high kurtosis values), more so than the other methods. This skewness is caused by an overestimation of the number of nearest neighbors in some cases, due to large values of either *d*_{std} or the parameter *α*. For the Voronoi Warnken–Reed method, there is a lack of a long tail and the skewness/kurtosis of the distribution tends more towards normality. However, the calculated mean PDAS with this method tends to underestimate the bulk-measured PDAS. While the maximum number of nearest neighbors (8 for *α* ≥ 1.2) is more realistic, a large percentage of dendrite cores are predicted to have only 3 nearest neighbors, even in the case of a large *α* parameter (48.6 pct for *α* = 2.0). It is also interesting that increasing the *α* parameter for the case of the Voronoi Warnken–Reed method tends to shift the slope of the probability distribution function without affecting either the minimum or maximum local dendrite arm spacings.

For comparison, the minimal spanning tree method (Figure 3) was also included in Table I. Not surprisingly, the mean distance of the connecting line segments is much shorter than the bulk calculated PDAS using Eq. [1] with *c* = 1. Remember that the MST method is composed of the shortest line segments to connect all dendrites. Both the MST standard deviation and kurtosis values are larger than the Voronoi tessellation method (for all *d*_{crit}) and the Voronoi Warnken–Reed method (for all *α*), indicating a wider distribution and a larger deviation of the distribution from normality (kurtosis = 3). Moreover, the distribution is skewed towards a larger tail at lower distances (negative skewness) unlike the other techniques, which again is associated with the selection of the shortest line segments to characterize the spacing.

Quantifying the coordination number and the local PDAS values using all FNNs identified by the Voronoi tessellation polygons (*d*_{crit} = 0) clearly overestimates both measures; mean PDAS is ∼10 pct off from the bulk-measured PDAS value and ∼20 pct of dendrite cores have more than 6 nearest neighbors. As the edge length threshold parameter increases, less nearest neighbors are identified and the calculated mean PDAS approaches the bulk-measured PDAS value (within 0.3 pct for *d*_{crit} = 0.12). For *d*_{crit} = 0.12, the majority of dendrite cores have 4 nearest neighbors (>50 pct), followed by 5 nearest neighbors (26.9 pct) and 3 nearest neighbors (17.3 pct). Moreover, the local PDAS distribution has a low skewness value (0.2) and a kurtosis of 2.9, indicating an approximately normal distribution. In general, the Voronoi tessellation-based technique with an edge length threshold criterion of *d*_{crit} = 0.12 tends to give the best agreement in terms of both bulk-measured PDAS and coordination number.

### 3.5 Correlation with Interdendritic Features

The relationship between the occurrence of interdendritic features (*e.g.*, pores or eutectic particles) and the local dendrite arm spacing (or distance from cores, *etc.*) can provide insight into the importance of quantifying the local spacings. We have examined how these metrics may relate to the formation of eutectic particles in this work by first segmenting the interdendritic particles and then computing probability distribution functions.

*etc.*). The threshold intensity was then selected by maximizing the difference in the mean intensity between the two distributions (eutectic particle and matrix). Then, a size threshold was enforced by discarding eutectic particles with less than 5 pixels (1 pixel ∼1.7

*μ*m,

*i.e.*, 5 pixels = 15.2

*μ*m

^{2}). As an example of the segmentation, Figure 10(a) shows a 1mm × 1 mm region from Figures 4 and 10(b) shows the corresponding binary image of the segmented eutectic particles (in white). While other segmentation techniques, such as region growing,[29] have been used to segment these interdendritic particles features in 3D serial slices, the method utilized within produced sufficient segmentation of the particles for the subsequent analysis.

The Euclidean distance to the nearest dendrite core and the nearest Voronoi vertex was then calculated for each pixel within the micrograph. The Euclidean distance is the distance from each pixel to the nearest feature, which in this case is either the centroids of the dendrite cores or the Voronoi vertices, and this metric is repeated over all pixels within the image to create a map. As an example, Figure 10(c) shows the Euclidean distance map for the same 1 mm × 1 mm area utilizing the dendrite core centroids identified in Figure 4. The darker intensity indicates closer Euclidean distances to the dendrite core and the lightest pixels between the dendrite cores actually correspond to the boundaries of the Voronoi tessellation.

*μ*m of the image boundaries were excluded to eliminate the possibility that dendrite cores just outside of the image field of view could affect the statistics. As can be seen from Figure 11(a), the left (right) blue line indicates the distance whereby all distances below (above) have a probability of having a eutectic particle that is lower (higher) than the global area fraction (red line),

*i.e.*, it is less (more) favorable for a eutectic particle to form. The transition distance of eutectic particle favorability is between 86 and 93

*μ*m,

*i.e.*, ~1/3 of the PDAS (248.4

*μ*m). This plot shows that it is not favorable for eutectic particles to form close to the primary dendrite core.

Figure 11(b) is a similar plot as a function of distance from the vertices of the Voronoi tessellation (see schematic). This plot was generated in a similar manner to Figure 11(a); a Euclidean distance map was first formed from the Voronoi vertices, then the boundary pixels within 100 *μ*m of the image boundaries were excluded, *etc.* There is an increased occurrence of eutectic particles at vertices, regardless of their distance from the dendrite core. This observation (along with the fact that the probability of occurrence is higher than in Figure 11(a) by almost 2 pct) suggests that solute is forced near the Voronoi vertices, thereby increasing the probability of eutectic particle occurrence. The transition distance in this plot is between 67 and 90 *μ*m,* i.e.*, at ~1/3 of the PDAS. While this analysis shows the preferential formation of eutectic particles based on the local distances, correlation with the size of particles is also important.

*A*

_{50}= 410

*μ*m

^{2}, which refers to the eutectic particle size where 50 pct of the eutectic particle area lies above/below this size. There is a noticeable tendency for the larger particles (

*A*>

*A*

_{50}) to form further away from the dendrite core and closer to the Voronoi vertices, while the smaller eutectic particles (

*A*<

*A*

_{50}) can form at all distances. However, it is difficult to quantitatively tell from the following plot what the preference is for smaller or larger particles as a function of distance. Therefore, to further quantify this relationship with respect to the size of the particles, the probability associated with a eutectic particle pixel belonging to either a small or large particle is calculated in Figure 13. Interestingly, in Figure 13(a), at distances closer to the dendrite cores, there is a clear preference for smaller particles (

*A*<

*A*

_{50}) to form over larger particles (

*A*>

*A*

_{50}). At a distance of 84.5

*μ*m (∼1/3 PDAS), as denoted by the solid line, there is a crossover in the probability function and larger particles are statistically favored to form over smaller particles. In the case of distances from the Voronoi vertices, there is a similar behavior except that

*larger*particles are favored at smaller distances (closer to Voronoi vertices). The crossover in the probability functions occurs at 79.3

*μ*m (∼1/3 PDAS again). At distances greater than this, there is not as definitive of a trend as with the dendrite cores,

*i.e.*, in some cases, there is a greater probability for smaller particles to form and, in some cases, for larger particles to form. Clearly, the distance from the dendrite cores and, hence, the local PDAS affect the probabilities of interdendritic particles to form, though. In a similar manner, it is anticipated that a similar relationship may be associated with shrinkage porosity, gas porosity, and other interdendritic defects.

## 4 Conclusions

Characterizing the PDAS in directionally solidified microstructures is an important step for developing process–structure–property relationships by enabling the quantification of (i) the influence of processing on microstructure and (ii) the influence of microstructure on properties. Thin-walled directionally solidified structures (*e.g.*, a turbine blade) require new approaches for characterizing the dendrite arm spacing and the microstructure. In this work, we utilized a new Voronoi-based approach for spatial point pattern analysis that was applied to an experimental dendritic microstructure. This technique utilizes a Voronoi tessellation of space surrounding the dendrite cores to determine nearest neighbors and the local PDAS. In addition, we compared this technique to a recent distance-based technique, the Warnken–Reed method, and a modification to this using Voronoi tessellations, along with the minimal spanning tree method. Moreover, a convex hull-based technique was used to include edge effects for such techniques, which can be important for thin specimens. These methods were used to quantify the distribution of local PDASs as well as their spatial distribution for an experimental directionally solidified superalloy micrograph. Last, eutectic particles were segmented to correlate distances from dendrite cores and Voronoi vertices to the occurrence and size of these interdendritic features. Interestingly, with respect to the distance from the dendrite core, it was found that there is a greater probability of occurrence of large eutectic particles (>410 *μ*m) over small particles at distances greater than ~1/3 of the bulk-measured PDAS. This systematic study of the different techniques for quantifying local PDASs, and their effect on microstructure, can be an important step for correlating with both processing and properties in single-crystal nickel-based superalloys.

## Notes

### Acknowledgments

MAT would like to acknowledge AFOSR for support for this research through contract FA9550-12-1-0135 (PM: Dr. David Stargel, AFOSR/RSA). MAT would like to acknowledge support from the U.S. Army Research Laboratory (ARL) administered by the Oak Ridge Institute for Science and Education through an interagency agreement between the U.S. Department of Energy and ARL.

### References

- 1.R.C. Reed:
*The Superalloys: Fundamentals and Applications*. Cambridge University Press, Cambridge, 2006.Google Scholar - 2.Pollock T.M., Tin S., Propuls J. (2006) . Power 22(2):361–374CrossRefGoogle Scholar
- 3.Whitesell H.S., Overfelt R.A. (2001) . Mater. Sci. Eng. A 318(1–2):264–276CrossRefGoogle Scholar
- 4.Elliott A.J., Tin S., King W.T., Huang S.C., Gigliotti M.F.X., Pollock T.M. (2004) . Metall. Mater. Trans. A 35A:3221–3231CrossRefGoogle Scholar
- 5.Melo M., Rizzo E.M.S., Santos R.G. (2005) . J. Mater. Sci. 40(7):1599–1609CrossRefGoogle Scholar
- 6.Lamm M., Singer R.F. (2007) . Metall. Mater. Trans. A 38A:1177–1183CrossRefGoogle Scholar
- 7.Brundidge C.L., Vandrasek D., Wang B., Pollock T.M. (2012) . Metall. Mater. Trans. A 43A:965–976CrossRefGoogle Scholar
- 8.Quested P.N., McLean M. (1984) . Mater. Sci. Eng. A 65:171–180CrossRefGoogle Scholar
- 9.Wills V.A., McCartney D.G. (1991) . Mater. Sci. Eng. A 145:223–232CrossRefGoogle Scholar
- 10.McCartney D.G., Hunt J.D. (1981) . Acta Metall. 29(11):1851–1863CrossRefGoogle Scholar
- 11.Hui J., Tiwari R., Wu X., Tewari S.N., Trivedi R. (2002) . Metall. Mater. Trans. A 33:3499–3510CrossRefGoogle Scholar
- 12.Wang W., Lee P.D., McLean M. (2003) . Acta Mater. 51(10):2971–2987CrossRefGoogle Scholar
- 13.J.D. Miller and T.M. Pollock: in
*Superalloys 2012*, John Wiley & Sons, Inc., Hoboken, 2012, pp. 653–62.Google Scholar - 14.Brundidge C.L., Miller J.D., Pollock T.M. (2011) . Metall. Mater. Trans. A 42A:2723–2732CrossRefGoogle Scholar
- 15.Wilson B.C., Cutler E.R., Fuchs G.E. (2008) . Mater. Sci. Eng. A 479(1-2):356–364CrossRefGoogle Scholar
- 16.Flemings M.C. (1974) . Metall. Trans. A 5A:2121–2134CrossRefGoogle Scholar
- 17.Jacobi H., Schwerdtfeger K. (1976) . Metall. Trans. A 7A:811–820CrossRefGoogle Scholar
- 18.Tewari S.N., Weng Y.H.S., Ding G.L., Trivedi R. (2002) . Metall. Mater. Trans. A 33:1229–1243CrossRefGoogle Scholar
- 19.Paul U., Sahm P.R., Goldschmidt D. (1993) . Mater. Sci. Eng. A 173:49–54CrossRefGoogle Scholar
- 20.M.A. Tschopp, A.L Oppedal, J.D. Miller, M.A. Groeber, A.H. Rosenberger, and K.N. Solanki: in
*Characterization of Minerals, Metals and Materials 2013*, John Wiley & Sons, Inc., Hoboken, 2013, pp. 299–310.Google Scholar - 21.Warnken N., Reed R.C. (2011) . Metall. Mater. Trans. A 42A:1675–1683CrossRefGoogle Scholar
- 22.Warnken N., Reed R.C. (2011) . IOP Conference Series: Mater. Sci. Eng. 27:1–5Google Scholar
- 23.Dussert C., Rasigni G., Rasigni M., Palmari J., Llebaria A. (1986) . Phys. Rev. B 34(5):3528–3531CrossRefGoogle Scholar
- 24.Billia B., Jamgotchian H., Thi H.N. (1991) . Metall. Trans. A 22A:3041–3050CrossRefGoogle Scholar
- 25.Peng P., Li X.Z., Su Y.Q., Liu D.M., Guo J.J., Fu H.Z. (2013) . J. Mater. Res., 28(5):740–746CrossRefGoogle Scholar
- 26.J.D. Miller: Ph.D. Thesis, University of Michigan, 2011.Google Scholar
- 27.Tschopp M.A., Groeber M.A., Fahringer R., Simmons J.P., Rosenberger A.H., Woodward C. (2010) . Scr. Mater. 62(6):357–360CrossRefGoogle Scholar
- 28.Tschopp M.A., Groeber M.A., Simmons J.P., Rosenberger A.H., Woodward C. (2010) . Mater. Charact. 61(12):1406–1417CrossRefGoogle Scholar
- 29.Tschopp M.A., Groeber M.A., Fahringer R., Simmons J.P., Rosenberger A.H., Woodward C. (2010) . Modell. Simul. Mater. Sci. Eng. 18:025014CrossRefGoogle Scholar